Presentation on theme: "Presentation downloadable from www.tececo.com 1 TecEco - Carbonating and Hydraulic Mortars Earthship Brighton (UK) – The first building utilising TecEco."— Presentation transcript:
Presentation downloadable from www.tececo.com 1 TecEco - Carbonating and Hydraulic Mortars Earthship Brighton (UK) – The first building utilising TecEco eco-cement mortars The presentation is always downloadable from the TecEco web site if you missed something. I will not go into the chemistry of the various binders in my presentation in detail but my paper in the proceedings does. John Harrison B.Sc. B.Ec. FCPA.
Presentation downloadable from www.tececo.com 2 Introduction Mortar has traditionally held walling units together and is still the choice of many builders. The requirements for proper carbonation when carbonating lime or the new eco-cement magnesian mortars are used are however poorly understood, especially in the English speaking world. This presentation compares carbonating and hydraulic mortars and discusses: –The impact of physical factors such as aggregate size, grading and moisture. The role of aggregates for proper carbonation is considered from a theoretical point of view and in terms of best practice from the past. The presentation concludes that sands suitable for hydraulic mortars are not suitable for carbonating mortars and visa versa and points out deficiencies in the current standards and codes of practice that do not recognize this. A new direction is suggested that combines the best practice from the past with that of the present.
Presentation downloadable from www.tececo.com 3 Introduction (2) Given –The increasing popularity of 1:1:6 through to 1:3: 10-12 mortars –The possibility of carbon credits for sequestration it is essential that the industry get its act together. –There would be significant potential commercial and technical benefit of cutting through the dogma and providing a proper scientific basis for formulation and for codes of practice that recognise the differing requirements of hydraulic and carbonating mortars, particularly for aggregates and curing conditions. If either lime mortars, PC - lime mortars or eco-cement mortars were optimised for carbonation there would be significant sustainability and other benefits.
Presentation downloadable from www.tececo.com 4 Introduction – Eco-Cement Mortars The new magnesian mortars developed by TecEco set by absorbing carbon dioxide in porous substrates such as mortars Eco-cements add a new dimension as they are easier to use, do not appear to suffer the segregation problem of mixed lime PC mortars and as a carbonating mortar potentially develop greater strengths including bond strength to bricks because of the unique microstructure attributable to the highly acicular nature of the hydrated magnesium carbonates formed. They develop higher early tensile strengths and are also more acid resistant, yet retain the benefits of self healing attributed to lime mortars. The new eco-cement mortars should theoretically provide the plasticity required with coarser aggregates and may overcome the tendency in the trade to formulate for ease of use rather than properties.
Presentation downloadable from www.tececo.com 5 Sustainability Sustainability is a direction not a destination. Our approach should be holistically balanced and involve –Everybody, every process, every day. Mineral Sequestration Eco-cements in cities + Waste utilization Geological Seques- tration Emissions reduction through efficiency and conversion to non fossil fuels + +
Presentation downloadable from www.tececo.com 6 Huge Potential for Sustainable Materials in the Built Environment The built environment is made of materials and is our footprint on earth. –It comprises buildings and infrastructure. Building materials comprise –70% of materials flows (buildings, infrastructure etc.) –40-45% of waste that goes to landfill (15 % of new materials going to site are wasted.) Reducing the impact of the take and waste phases of the techno-process. –By including carbon in materials they are potentially carbon sinks. –By including wastes for physical properties as well as chemical composition they become resources C C C C C Waste
Presentation downloadable from www.tececo.com 7 Background Until the beginning of this century most buildings were constructed with lime and hydraulic lime mortars and many still stand as testament to their quality. –Examples include many Roman lime mortars such as in Hadrians wall built nearly 2000 years ago (122 AD) and the Tower of London built some 900 years ago. Portland cement mortars until recently had taken over the mortar market in English speaking countries, whereas in many other parts of the world such as Slovenia where PC mortars are banned, lime mortars never went out of use. There is currently a trend back to the use of lime mainly for the plasticity introduced to mixes. There will potentially be a rush towards carbonating lime mortars if carbon credits became available for proven sequestration The masonry industry needs to prepare itself for such a commercial opportunity.
Presentation downloadable from www.tececo.com 8 Background (2) The requirements of mortars of varying degrees of hydraulicity and carbonation potential are poorly understood The lack of science appalling amongst engineers and the trade in the UK, USA and Australasia. The way hydraulic mortars, carbonating mortars or pozzolans are used together is not generally optimised in the English speaking world and there is much controversy. All over the world carbonating mortars are not fairly considered by standards designed for hydraulic cements.
Presentation downloadable from www.tececo.com 9 Background (3) The focus is on ease of use rather than end result –For example in the most used 1:1:6 or 1:2:9 (pc, lime, aggregate) type mixes, the aggregates used are generally much too fine and well graded for the lime to serve as much other than a plasticiser. Hydraulic limes are rarely used and poorly understood Little advantage is taken of pozzolanic wastes except in Europe, Asia and the USA.
Presentation downloadable from www.tececo.com 10 The Historic Background The historic record is confusing A thorough analysis is overdue –based on fundamentals –that is not clouded by inappropriate standards. Although good mortars from the past have lasted through the ages there have also been many failures as well. The biggest problem in trying to discern best practice from the past is that historic mortars formulations are many and varied although underlying many of them there exists some common lessons for the present that are in agreement with good science.
Presentation downloadable from www.tececo.com 11 The Historic Record Most old carbonating lime mortars are a mix of lime putty, lime sand, and grit. –Generally a greater proportion of lime was used for sandstone or sedimentary rocks and a harder mortar used for granite or impervious rocks. According to Benjamin Herring, editor in chief of constructor magazine The Romans had two distinct types of concrete mortar. –One was made with simple lime and river sand, mixed at a ratio of three parts sand to one part lime. –The other type used pozzolan instead of river sand and was mixed at a ratio of two parts pozzolan to one part lime.
Presentation downloadable from www.tececo.com 12 Carbonating Mortars Used by The Romans The oldest record: Book II, chapter IV of the Ten Books of Architecture by Vitruvius Pollio . –According to Vitruvius the best (sand) will be found to be that which crackles when rubbed in the hand, while that which has much dirt in it will not be sharp enough. Again: throw some sand upon a white garment and then shake it out; if the garment is not soiled and no dirt adheres to it, the sand is suitable Vitruvious was talking about gritty sand with no fines. The 16th century architect Andrea Palladio is renowned for "The Four Books of Architecture –translated into English in the early 18th century –used as a principal reference for building for almost two centuries (Palladio, Isaac Ware translation, 1738). In the first book Palladio says, "the best river sand is that which is found in rapid streams, and under water-falls, because it is most purged". In other words, it is coarse. Compare this with most sand for use in mortar today.
Presentation downloadable from www.tececo.com 13 Advantages of Carbonating Mortars Modern Portland cement mortars and even some fully hydraulic lime mortars –Set too hard and do not self-heal. –Tend to crack with any movement and let water in. Once the water is in they are so tight they do not let it out again as they cannot breathe leading to further problems. Advantages of carbonating mortars include: –Plasticity –They are much more forgiving. As all buildings move, especially those built pre 1900, many of which had less solid foundations, this property alone is reason enough to use them. A carbonating component is required for crystalline bridging of cracks that develop through movement. Global warming is a major issue and the huge potential in the built environment for sequestering carbon cannot be ignored. There is an urgent need to reconsider the merits of properly carbonating mortars in the context of global warming.
Presentation downloadable from www.tececo.com 14 Carbonating Mortars in the Context of Global Warming Cementitious materials that go the full thermodynamic cycle gaining strength by carbonation offer tremendous potential because the CO2 chemically released during manufacture can be recaptured resulting in significant overall sequestration. –To put the tonnages involved into context, in 2004, by calculation from clay brick and concrete block production, Australians used about 300,000 tonnes of Portland cement to make mortars. Roughly only 25% of this cement carbonates so 225,000 tonnes of CO2 are released assuming emissions are taken to be roughly one tonne of CO2 per tonne of cement. If lime or high magnesian eco-cements were used in Australia the reduction in CO2 emissions would be a significant 225,000 tonnes. Australia is only about 1.4% of the economic world so globally the figure is significant.
Presentation downloadable from www.tececo.com 15 Other Sustainable Benefits of Carbonating Mortars The bulk density is lower than Portland cement enabling fuel savings during distribution. Buildings constructed with all but the strongest lime and eco-cements can also easily be altered and recovered masonry reused. –In contrast bricks held together with Portland cement mortars usually cannot easily be recycled as the mortar is too strong. –The production of bricks and masonry units is an energy intensive process and the savings involved as a result of more efficient recycling would be considerable.
Presentation downloadable from www.tececo.com 16 Advantages Summary Sustainability with less net emissions The accommodation of minor and thermal movement without damage. The avoidance of expansion joints. Improved insulation and avoidance of cold bridging. Reduced risk of condensation. Low risk of salt staining. Alterations can be effected easily and masonry revised. Lower pH Masonry life is increased. Masonry can more easily be cleaned and reused. More resistant to freeze thaw and sulphate. Reduced calcium aluminate content & reactions with sulphate in stone. Lower alkalinity and reactions with stone, particularly sandstone Better bond to acidic or more neutral rocks like sandstone. Buildings which themselves breathe are healthier to live in.
Presentation downloadable from www.tececo.com 17 Disadvantages of Carbonating Mortars??! Lea (The Chemistry of Cement and Concrete) Mortar taken from buildings many hundreds of years old, if uninjured, is found to consist mainly of calcium hydroxide, only the external portion has been converted to carbonate. –Note however that the lack of carbonation of some old mortars can be explained as a function of low porosity due to poor aggregate selection rather than due to an innate inability of lime to carbonate. Lime type carbonating mortars are considered by many as too weak for copings, chimneys and other exposed work. –As minerals such as nesquehonite found in eco-cement mortars are micro structurally stronger this problem may be overcome by substitution with magnesia as in eco-cements. Currently there is also a danger regarding use in frost prone months. –This is however not the fault of the binder so much as because the fine sands used not only dont let air in for carbonation – they dont let moisture out. Lime mortars are subject to attack by acid rain. –Fortunately eco-cements appear to be much more acid resistant. The thermodynamics and kinetics is complex however the evidence is that no potholing or caving is ever found in magnesium carbonate country. Chlorides and sulphates attack lime and Portland cement mortars –Chlorides and sulphates are rendered chemically inactive and cementitiously useful by the magnesia in eco-cement type formulations. –As these salts are common in some rocks and bricks and certainly in city environments, particularly near the sea or where salt is used on roads, eco- cements should be considered for this reason alone.
Presentation downloadable from www.tececo.com 18 The Right Sands & Aggregates The major problem with nearly all mortars today is that the same sands tend to be used for all of them regardless of the incongruous requirements for proper compaction or carbonation. Carbon dioxide is pervasive in the atmosphere at about 380 ppm and rising. –For carbonation to occur in either lime, blended lime PC or eco-cement mortars the mortar must be able to breathe. By breathing vapors must be able to pass into the mortar through it and out of it. –Carbonation reactions however generally occur in the aqueous phase much more quickly than in the gas phase and thus water vapor is also necessarily present. Coarse sands fractions are required in the aggregates used and this is unfortunately poorly understood except by some in the restoration industry. In contrast, for Portland cement mortars to gain strength the main requirement is for a low water binder ratio. For this relatively fine sands that are rounded and compact well are required that minimise the amount of cement required for full cover.
Presentation downloadable from www.tececo.com 19 The Right Sands & Aggregates (2) The right sands should be clean and well graded, ranging from fine to coarse, and be gritty in texture. Generally specify washed sharp sand with 3-4 mm grit (where the joints allow) and not too high a proportion of fines is suitable A well-graded masonry sand that has a range of grain sizes from fine to coarse is best. –The coarsest grains should however be no more than 1/3 the depth of the mortar between bricks for easy laying. Beware of artificially crushed stone dusts (especially limestone). –These cause shrinkage problems, are weak and have poor adhesion. Although logical as a ramification of the chemistry the requirements of sand seems to be poorly understood except by a few within the restoration fraternity
Presentation downloadable from www.tececo.com 20 Binder Types and Manufacture Portland Cement –Portland cements are similar to hydraulic limes as they were derived from them by calcining limestone with clay at higher temperatures of around 1450oC. The main hydrating mineral present include alite, belite, tri-calcium aluminate and calcium alumino ferrite. Tec-Cements –Tec-cements (5-15% MgO, 85-95% OPC) contain more Portland cement than reactive magnesia. Reactive magnesia hydrates in the same rate order as Portland cement forming Brucite which uses up water reducing the voids:paste ratio, increasing density and possibly raising the short term pH. Reactions with pozzolans are more affective. After all the Portlandite has been consumed Brucite controls the long term pH which is lower and due to its low solubility, mobility and reactivity results in greater durability. –Other benefits include improvements in density, strength and rheology, reduced permeability and shrinkage and the use of a wider range of aggregates many of which are potentially wastes without reaction problems. Portland and tec-cements are not discussed further as they are not recommended for mortars)
Presentation downloadable from www.tececo.com 21 Hydraulic Limes –Louis Vicat (1786-1861) introduced the term "hydraulic lime" in place of the earlier term "water lime" used by Joseph Smeaton of Eddystone lighthouse fame and others and classified limes according to their hydraulicity. Hydraulic limes are not Portland cement but have many characteristics that are similar as Portland type cements are derived from them. The decarbonation of lime is greatly favoured by intimate mixing with clay minerals. –When heated at moderate temperatures clay impurities in limestone dehydroxylate forming in the case of kaolin metakaolin and generally kandoxi (dehydroxylated, activated mixed clays) Some reactions also occur between the kandoxi and lime producing calcium silicate hydrate precursors which are hydraulic and set when they hydrate including belite, aluminate and ferrite phases. Gehlenite has also been reported. A hydraulic cement contains lime, silica and alumina and hardens by hydration and most of the minerals formed and are therefore hydraulic. The term Kandoxi was introduced by Joseph Davidovits of geopolymer fame for mixed de hydroxylated (dehydrated) clays to get over the rather loose use of the term metakaolin. See http://www.geopolymer.org
Presentation downloadable from www.tececo.com 22 Partially Hydraulic Limes Partially hydraulic limes have residual lime and are usually slaked with just enough water to convert the quicklime left to calcium hydroxide, but not so much that a chemical set begins. –Hardening occurs by carbonation of the remaining slaked lime as well as reactions between it and unreacted kandoxi and calcium silicates forming calcium silicate/aluminate hydrates. –At around 40% silica/alumina maximum strengths are achieved and there is no 'free' hydroxide to carbonate. The degree of hydraulicity of mortars effects many characteristics. –By selecting an appropriate ratio of clay to limestone mortars that carbonate or set hydraulically to a varying extents can be designed for particular application requirements such as setting time, strength, colour, durability, frost resistance, workability, speed of set in the presence of water, vapour permeability etc. Hydraulic lime mortars are arguably better than PC mortars and PC non hydraulic lime mortars and are sought after in the restoration industry In the context of global warming it may be better to focus on mortars that can gain strength through carbonation such as partially hydraulic lime mortars, non hydraulic or carbonating lime mortars or high lime PC blends or mortars made using the new eco-cements developed by John Harrison of TecEco.
Presentation downloadable from www.tececo.com 23 Non Hydraulic Lime Mortars Non hydraulic lime mortars rely on carbonation for strength development. –When reactive lime carbonates it follows Ostwalds law forming vaterite, aragonite and calcite in that order. Ca(OH)2 + CO2 CaCO3 + H2O –The reaction is thought to be through solution and the first step is the dissolution of calcium hydroxide followed by reaction with dissolved carbon dioxide. Ca(OH)2 Ca2+ + 2OH- Ca2+ + 2OH- + CO2 CaCO3 + H2O Commonly available lime is generally fired at between 850 and 1100oC and then slaked –is relatively pure as manufacturers tend to pick or sieve out any sintered clinker like lumps where it has reacted with impurities. –Although it is not the best available for use in lime mortars because it is often slightly hard burned through the overuse of flash calciners, it is what is being used for most blended mortar formulations such as 1:1:6 or 1:2:9 (PC:lime:sand).
Presentation downloadable from www.tececo.com 24 Non Hydraulic Eco-Cement Mortars Instead of calcium hydroxide as the main ingredient, reactive magnesia (MgO) is used which first hydrates forming brucite (Mg(OH)2) and then carbonates forming an amorphous phase, lansfordite and nesquehonite. MgO Mg(OH)2 MgCO3.5H2O MgCO3.3H2O ??????? and maybe eventually MgCO3 The reaction is also probably through solution but favours the formation of hydrated carbonates as the highly charged Mg++ ion in water strongly attracts polarised water molecules around it which are not easily removed and therefore incorporated in the new carbonate molecules when formed.
Presentation downloadable from www.tececo.com 25 The Relevance of Modern Standards Lime mortar standards were developed at the time that Portland cement was being introduced as a key material in mortars. –As a consequence most of the curing conditions were established on the basis of the hydration requirements of Portland cement (minimum paste for cover) rather than the requirements of carbonation. It should be obvious that lime mortars cannot perform as well under these conditions. For example: –Mechanical testing at 28 days. Lime and eco-cement mortars take longer. Lime mortars require carbon dioxide for the carbonation reaction. –Although the presence of moisture will facilitate the carbonation reaction of the lime and crystallization of the resulting calcite crystals, too much moisture, as under the BS conditions, will slow down the reaction. –This can be explained by considering that all the exposed surfaces of the lime mortar are covered with a layer of liquid water and that the CO2 has to diffuse through it before it can reach the lime surface.
Presentation downloadable from www.tececo.com 26 Particles Size Specification in Standards Jordan, J.W. The Conservation and Strengthening of Masonry Structures. in Proceedings of the 7th Australasian Masonry Conference. 2004. Newcastle, New South Wales, Australia: University of Newcastle, Australia. Sand grading for permeable mortar compared to BS 1200 and AS 3700-991 recommendations (Note that a mortar for successful carbonation barely falls within the ranges specified by the standards. A more suitable mortar would most likely fall without.)
Presentation downloadable from www.tececo.com 27 Improving The Status Quo One has to consider why in the face of science and the historic record the standards allow the use of such inappropriate aggregates for carbonation and apply such unfair advantages in tests to hydraulic cements. Perhaps the answer lies in a misguided belief that the only answer is Portland cements and that the only sand sold should optimise hydraulic setting. It is time cement companies dropped the philosophy of if its grey its great and all we make goes out the gate. –A small number are now making lime as well as Portland cement –As The only enduring business is the business of change. Perhaps the cement industry need to understand that they are in the mineral composite business and that some minor diversification could actually be more profitable, particularly if there were opportunities for carbon credits through sequestration in the built environment. –Adopting new technologies will result in new products and may mean new resources are defined many of which are wastes. New products create new market share. Pilzer, P.Z., Unlimited Wealth - The Theory and Practice of Economic Alchemy. 1 ed. 1990: Crown Publishers
Presentation downloadable from www.tececo.com 28 Meeting the Sustainability Challenge There are new demands for sustainability being placed upon the industry. With the advent of Kyoto as a treaty there could even be money to be made from carbon credits if mortars containing lime or magnesia (as in eco-cements) were allowed to carbonate properly. The new eco-cements from TecEco are exciting as they are potentially far more sustainable. –They contain relatively high proportions of MgO that will first hydrate and then carbonate. –The production of magnesia can be achieved using an efficient low temperature process that can use waste heat or free solar energy. The capture of CO2 during this process would result in sequestration on a massive scale. The magnesia used is relatively fine and like lime, markedly improves rheology. MgO mortars also appear to also be more tolerant of some clays –Actually exhibiting more strength in their presence and this could be an advantage in terms of being able to utilise sands without the cost of washing and disposal problems associated with the clay fines fraction. –For mud brick manufacture using soils rather than sands it is a definite advantage. A case study on mud bricks using a high clay soil is on the TecEco web site. Because Mg++ is a small and highly charged ion it tends to cause polar water molecules to orientate in layers around it introducing a shear thinning property improving for example anti sag properties in mortars as would methyl cellulose. Nesquehonite is the main observable carbonate and forms star like acicular growths which adds to microstructural strength. Fibrous carbonate growth may also improve bonding with brick, tiles and various walling substrates. Significant quantities of binder are produced. –The larger proportion of magnesium carbonates formed is CO 2 and water
Presentation downloadable from www.tececo.com 29 CO 2 Abatement in Eco-Cements Eco-cements in porous products absorb carbon dioxide from the atmosphere. Brucite carbonates forming lansfordite, nesquehonite and an amorphous phase, completing the thermodynamic cycle. No Capture 11.25% mass% reactive magnesia, 3.75 mass% Portland cement, 85 mass% aggregate. Emissions.37 tonnes to the tonne. After carbonation. approximately.241 tonne to the tonne. Portland Cements 15 mass% Portland cement, 85 mass% aggregate Emissions.32 tonnes to the tonne. After carbonation. Approximately.299 tonne to the tonne..299 >.241 >.140 >.113 Bricks, blocks, pavers, mortars and pavement made using eco-cement, fly and bottom ash (with capture of CO 2 during manufacture of reactive magnesia) have 2.65 times less emissions than if they were made with Portland cement. Capture CO 2 11.25% mass% reactive magnesia, 3.75 mass% Portland cement, 85 mass% aggregate. Emissions.25 tonnes to the tonne. After carbonation. approximately.140 tonne to the tonne. Capture CO 2. Fly and Bottom Ash 11.25% mass% reactive magnesia, 3.75 mass% Portland cement, 85 mass% aggregate. Emissions.126 tonnes to the tonne. After carbonation. Approximately.113 tonne to the tonne. For 85 wt% Aggregates 15 wt% Cement Greater Sustainability
Presentation downloadable from www.tececo.com 30 Conclusion Insufficient intelligent work has been done on the merits of various mortars and aggregates that are suitable for them –evident by the confusion and infiltration of art rather than science in the engineering literature. –This sad state of affairs is at its worst in relation to suitable aggregates (sands). The standards offer little real guidance and as they become more performance based they will not do so and the codes of practice and guides could certainly do with some improving. Sands specified for concrete tend to be used for mortars regardless of whether they are meant to set hydraulically, by carbonation or a mix of both. As the requirements of sand for carbonation are quite difference to those for hydraulic setting, and because of the increasing popularity and need for carbonating mortars for restoration and sustainability reasons urgent work needs to be undertaken to distinguish sands based on the end use and get away from one sock fit all approach of standards and informational literature. –The requirements for totally hydraulic limes and all PC mortars is to minimise the amount of water for hydraulic strength and maximise compaction and for this purpose aggregates that require grading and relatively fine rounded sands to minimise voids are required. –For carbonating mortars on the on the hand the mortars must breathe requiring a coarse fraction to cause physical air voids and some vapour permeability. Because of the differing requirements of aggregates (sand) it may be better not to mix hydraulic and carbonating mortars. Unfortunately however carbonating lime mortars do not set quickly enough and so PC is added wherein there is a need to compromise. –Air entraining agents and plasticisers partially solve the problem but care needs to be exercised in their use as there is a tendency to overdose with air entraining agents in particular as they give workability, but detrimentally form under brick bubble layers and weaken bond. –Surely a purely mineralogical and physical approach would be better.
Presentation downloadable from www.tececo.com 31 Conclusions (2) The new TecEco eco-cement magnesian mortars hold the promise of overcoming the problems associated with using only carbonating lime mortars such as rate of strength development, lack of plasticity with coarse sands and bond strength. Global population is expanding as rapidly as ever, there is a need to build millions of new homes over the coming years; however environmental issues are becoming more important. The introduction of a carbon tax, or legislation setting targets for recycling of buildings could reduce the demand for Portland cement and the new TecEco eco-cements and lime mortars will become more popular. Current practice is to add lime to mortars for plasticity and no other reason. Given the urgency of doing something about global warming it is about time the industry optimized the benefits of using carbonating and blended carbonating mortars. The best results will be obtained by combining some of the techniques of the past (carbonating mortars and mortars and walls that breathe) with those of the present (vents, vapor barriers, double skin walls and damp courses). More research needs to be done in this area, more work is required to develop the relevant codes of practice, and most importantly, considerable effort will need to be taken to disseminate the findings to people in the industry.